IOSR Journal of Mechanical and Civil Engineering (IOSR-JMCE) e-ISSN: 2278-1684,p-ISSN: 2320-334X, Volume 7, Issue 1 (May. - Jun. 2013), PP 12-19 www.iosrjournals.org

Experimental Evaluation of the Effect of Thread Angle on the Fatigue Life of Bolts Er. Shuhaib Mushtaq* , Dr. Nazir Ahmad Sheikh** *Research Scholar, Department of Mechanical Engineering, National Institute of Technology, Srinagar , India ** Assistant Professor, Department of Mechanical Engineering, National Institute of Technology, Srinagar, India

Abstract :

I.

Introduction

12 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts been investigated by many researchers such as Maduschka[13] and Birger[14] and has been fully reviewed by Kenny and Patterson [15, 16]. One theory for the load distribution is provided by Sopwith[17] modified later by Stoeckly and Macke [18]. The load distribution is given by: (2.1)

is given by: =

(2.2)

Where Kt is the stress concentration factor for the periodic notch embodied by the thread. This is treated as a single notch by considering an effective depth, t*, instead of the actual depth t ( 0.6495p for ISO standard) of the thread profile using t*= t, where

is the correction factor and is calculated as follows [20]: (2.3)

The bending stress

can be calculated using Heywood‘s method [21] which is based on the load distribution

given by Eq. (2.1). According to this method

is obtained using. (2.4)

Where , For ISO thread, e 0.4278p, r

,b

s The overall stress is obtained from a combination of

and

. This must be done with care, since the two

stresses do not occur at the same point. One of the appropriate combinations of these two stresses has been given by Heywood [22] (2.5) Where m= [(60-β)/44]2. The fatigue life, or endurance, of a material refers to the number of repeated cycles of loading (N) that a material will undergo before it fails. N will depend on the particular set of loading conditions. However, the general rule of thumb is that the higher the fatigue stress levels, the few number of loading cycles are required to cause failure. In most well designed bolted joints, however, fatigue failure will occur under high cycle loading. Fatigue data is most commonly presented in terms of S-N curves (maximum stress versus the number www.iosrjournals.org

13 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts of cycles), as shown in "Fig.1" The material undergoes a definite fatigue limit. That is, it may withstand infinite cycles of loading without failing, as long as the applied stress is less than the fatigue limit. Although S-N curves are often produced based on tension loading

Fig.1:S-N Curve for varying magnitude of life altering stresses. Source[1]

Fig.2: Effect of geometrical stress concentration on fatigue Source [23]

Along the axis of the fastener, it is important to recognize that if the fastener is subjected to some other form of stress as well as tension, its fatigue life will be adversely affected. Shear stress for example, would make it more susceptible to fatigue. There are many factors that will affect the fatigue life, each resulting in a different S-N curve. The major factors in order of importance that affect fatigue life are: 1. Shape of the connection. 2. Magnitude of stress excursions or variations. 3. Mean stress level. 4. Choice of material. In most structures, fatigue cracking usually initiates at a stress concentration. The stress concentration may by inherent in the design, such as a fillet, hole, thread, or other geometrical feature, or the stress concentration can result from a manufacturing process, such as a rough surface finish or residual tensile stresses introduced by heat treatment. The effect of geometrical stress concentrations on fatigue is often studied by testing notched specimens. When a notch is present in a specimen under uniaxial loading, three effects are present: (1) there is an increase in concentration of stress at the root of the notch, (2) there is a stress gradient from the notch toward the centre of the specimen, and (3) a triaxial state of stress exists. The dramatic reduction in fatigue life of normalized 4340 steel sheet containing different types of stress concentrations is shown in "Fig.2" The effect of notches on fatigue strength is determined by comparing the S-N curves of notched and unnotched specimens. The data for the notched specimens are usually plotted in terms of nominal stress based on the net cross section of the specimen. The effect of the notch in decreasing the fatigue strength is reported as the fatigue strength reduction factor, or the fatigue notch factor,

(2.6) For metals that do not have a definite fatigue limit, the fatigue notch factor is based on the fatigue strength at a specified number of cycles. Values of the fatigue notch factor vary with the severity of the notch, the type of notch, the material, the type of loading, and the applied stress level. Notched fatigue data are also reported using a notch sensitivity factor, q: (2.7) www.iosrjournals.org

14 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts

This relationship compares the theoretical stress-concentration factor,

, to the fatigue notch factor,

. In this

relationship, a material that experiences no reduction in fatigue due to a notch will have a notch sensitivity factor of q=0, while one that experiences a reduction in fatigue up to the full theoretical value will have a notch sensitivity factor of q=1. The value of q is dependent on the material and the Radius of the notch root, as illustrated by the plots shown"Fig.2" in for steels.

Fig.3: Notch Sensitivity verses notch radius for steels. Source [24] The notch sensitivity factor, q, significantly decreases with smaller notch radii. Although this seems counterintuitive, it occurs because increases more slowly than with decreasing notch radius .For notches with large radii,

is almost equal to

for materials with small notches,

is less than

strength metals are less affected than high-strength metals by geometric discontinuities that reduce the fatigue resistance, because high-strength metals have a limited capacity for deformation and crack tip blunting. Because almost all fatigue failures start on a surface, the surface finish and Residual-stress state near the surface can have a profound effect on the fatigue strength. Since the early days of fatigue investigations, it was recognized that the fatigue life of a component is very dependent on the surface finish produced by machining or grinding operations, highly polished steel specimens perform much better in fatigue than even carefully machined surfaces. Further degradation in fatigue strength occurs for hot rolled and forged surfaces. Finally, when corrosion is introduced, the fatigue life can be seriously degraded. Parts that are formed at room temperature will contain residual stresses. For example, the surface of a part that was formed in tension will contain residual compressive stresses, and a surface that was in compression during forming will contain residual tensile stresses. Since fatigue always occurs under tensile loading, the surface with the residual tensile stresses will be the most prone to fatigue cracking. Similar to forming, some quenching operations during heat treatment can result in a tensile residual-stress pattern on the surface that will adversely affect fatigue strength. According to Gane [19] a cursory examination of the mean stress values for the different thread geometries shows that the results appear to fall into two sets, those with a flank angle of 60째or less (low strength) and those with angles of 90째 or over (high strength). There is no obvious consistent variation with either pitches or root diameter .This is confirmed by plotting the results. "Fig.4" shows the effect of flank angle on test specimens with constant thread pitch and root radius Although the scatter of results is large, a significant increase in strength clearly occurs between 60째and 90 ,the effect of thread pitch is less clear.

www.iosrjournals.org

15 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts Fig.4: Effect of thread flank angle on fatigue stress. Source [19]

II: Experimental Work The standard specimen with five different thread profiles means changing flank angles [47°, 55°, 60°, 90°, and 110°] with a similar pitch of 1.5mm having major diameter of 10mm and minor diameter of 8.38mm with coarse threads has been used for this work. The mechanical properties of the bolt material (mild steel) were obtained from a number of tensile tests. These properties were then used to select the appropriate amplitude of the reversed loading in fatigue tests. These properties are the following:  Yield strength, 170MPa, ultimate tensile strength, 265MPa; Young‘s modulus E =

  

207MPa, and Poisson‘s ratio ν = 0.3. The design of the standard specimen has been according to the following: The ends of the specimen were made of the form to suit the type of machine used and the material being tested. The grip ends of the specimens were made symmetrical about the axis of reduced test section. The forms of the test specimens rectangular or circular cross sections depends upon the nature of particulars required from the tests and naturally the form in which the material is available. Where fundamental fatigue properties are desired, circular cross sections are recommended.

2.1 Specimen Geometry , Testing Apparatus And Procedure All the test specimens employed for a fatigue determination shall have the same nominal dimensions as follows, shown in. "Fig.5" Total length-------150mm, Major diameter-------10mm, Minor diameter (threaded portion) ---------8.38mm, Threaded portion length -------------50mm

Fig.4: Testing Specimen Fatigue tests were conducted using R.R Moore fatigue testing machine. The tests were performed under the sinusoidal cyclic loading. A general view of the testing machine each load has been obtained by the product of the designated stress and the root area of the bolt. The stresses were selected between the ultimate strength of the bolt material, and . The endurance limit of the bolt material has been obtained from the S-N curve of the bolt material and was found to be 160MPa for mild steel bolts. The load obtained in this way was considered as the amplitude of a sinusoidal load applied to the specimen by the testing machine. The load fluctuated between 0 and . The number of cycles corresponding to the failure has been recorded as the fatigue life of the bolt under testing. The core stresses were calculated as These stresses were then used to compare the fatigue life of threaded bolts of different flank angles. The ―Fig‘‘ below shows the fatigue failed sample

III:

Experimental Data And Results www.iosrjournals.org

16 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts The experimental results are given in Table1and in the same way data has been manipulated for all the samples. The table shows the fatigue life of threaded specimens with different flank angles at different core stresses. The tests were performed on each profile with six samples i.e. total numbers of thirty experiments were performed on five profiles respectively, and it must be mentioned that all experimental data, have been used to draw all S-N curves shown in the results SAMPLE NUMBER

FLANK ANGLE (DEGREE)

APPLIED CORE STRESS (MPa)

FATIGUE LIFE CYCLES

I

47

106.67

584646

II

do

142.23

209426

III

do

177.79

104784

IV

do

213.35

54346

V

do

248.91

34711

VI

do

284.47

10320

Table1 Graph 1

www.iosrjournals.org

17 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts

IV.

Conclusion

The fatigue strength of threaded connections with various thread geometries, made from mild steel material has been measured. The core stress of different thread profiles with various flank angles varies between 106.67 and 284.47 MPa, and the results obtained by plotting the S-N Curves of various thread flank angles has been compared with the work of Gane [19] , the results obtained agreed well with his work. From the results obtained following conclusions can be derived: The fatigue strength of bolts appear to fall into two sets, those with a flank angle of 55° or less ( low strength ) and those with angles of 60° or over ( high strength ) under the constant pitch and applied core stress. From the S-N Curve of 60° flank angle specimens have approximately 10-20% higher fatigue life when compared with the S-N Curve of 90° flank angle specimens.

www.iosrjournals.org

18 | Page

Experimental Evaluation Of The Effect Of Thread Angle On The Fatigue Life Of Bolts [24] [25] [26] [27] [28] [29] [30]

M.R. Mitchell, Fundamentals of Modern Fatigue Analysis for Design, Fatigue and Fracture, Vol 19, ASM Handbook, ASM International, 1996 Bouwman, L.P., Gresnigt, A.M. and Dubois, G.A., ―European Recommendations for Bolted Connections with Injection Bolts,‖ ECCS-TC10 draft. M.A. Meyers and K.K. Chawla,‖ Mechanical Metallurgy—Principles and Applications‖, Prentice-Hall Inc., 1984 Bouwman, L.P.,‖ Bolted connections dynamically loaded in tension‖, ASCE, J. of the Structural Division, Vol. 108, No. ST, September 1982. Euro code 3: "Design of steel structures": ENV 1993-1-1: Part 1.1, General rules and rules for buildings, CEN, 1992 Frost, N.E., March, K.J., Pook, L.P., ―Metal fatigue‖, Oxford University Press 1974. G. H. Majzoobi, G. H. Farrahi, N. Habibi. , ―Experimental evaluation of the effect of thread pitch on the fatigu e life of bolts‖, International journal of Fatigue vol. 27(2005) 189-196.

www.iosrjournals.org

19 | Page

Experimental Evaluation of the Effect of Thread Angle on the Fatigue Life of Bolts

http://www.iosrjournals.org/iosr-jmce/papers/vol7-issue1/C0711219.pdf